#------------------------------------------------------------------------------
#$Date: 2019-09-09 10:30:34 +0300 (Mon, 09 Sep 2019) $
#$Revision: 218095 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/37/7233715.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7233715
loop_
_publ_author_name
'Xiaoxia Lin'
'Fangfang Zhang'
'Shilie Pan'
'Hongwei Yu'
'Fangyuan Zhang'
'Xiaoyu Dong'
'Shujuan Han'
'Lingyun Dong'
'Chunyan Bai'
'Zheng Wang'
_publ_section_title
;
 Ba4(BO3)3(SiO4).Ba3X (X = Cl, Br): new salt-inclusion borosilicate
 halides as potential deep UV nonlinear optical materials
;
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              4257
_journal_page_last               4264
_journal_paper_doi               10.1039/C4TC00079J
_journal_volume                  2
_journal_year                    2014
_chemical_formula_sum            'B3 Ba7 Br O13 Si'
_chemical_formula_weight         1309.81
_space_group_IT_number           186
_space_group_name_Hall           'P 6c -2c'
_space_group_name_H-M_alt        'P 63 m c'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_H-M   'P 63 m c'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   11.279(3)
_cell_length_b                   11.279(3)
_cell_length_c                   7.324(4)
_cell_measurement_reflns_used    1420
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      26.85
_cell_measurement_theta_min      4.17
_cell_volume                     806.9(5)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0764
_diffrn_reflns_av_sigmaI/netI    0.0316
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            9456
_diffrn_reflns_theta_full        27.40
_diffrn_reflns_theta_max         27.40
_diffrn_reflns_theta_min         2.08
_exptl_absorpt_coefficient_mu    19.407
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6755
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'face indexed'
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    5.391
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             1120
_exptl_crystal_size_max          0.184
_exptl_crystal_size_mid          0.065
_exptl_crystal_size_min          0.046
_refine_diff_density_max         2.031
_refine_diff_density_min         -1.329
_refine_diff_density_rms         0.242
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.05(7)
_refine_ls_extinction_coef       0.0020(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.103
_refine_ls_matrix_type           full
_refine_ls_number_parameters     53
_refine_ls_number_reflns         677
_refine_ls_number_restraints     13
_refine_ls_restrained_S_all      1.093
_refine_ls_R_factor_all          0.0365
_refine_ls_R_factor_gt           0.0322
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+30.7388P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0655
_refine_ls_wR_factor_ref         0.0684
_reflns_number_gt                639
_reflns_number_total             677
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            1000002.cif
_cod_data_source_block           PCOD1000002
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Hexagonal' was changed to
'hexagonal' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_sg_symbol_H-M      'P6(3)mc '
_cod_database_code               7233715
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z+1/2'
'x-y, -y, z+1/2'
'-x, -x+y, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1 Ba 0.3333 0.6667 0.1265(3) 0.0108(4) Uani 1 6 d S . .
Ba2 Ba 0.71016(10) 0.85508(5) -0.16899(13) 0.0164(3) Uani 1 2 d S . .
Ba3 Ba 0.05133(9) 0.52566(5) 0.48600(15) 0.0131(2) Uani 1 2 d S . .
Si1 Si 0.3333 0.6667 -0.2822(14) 0.0146(19) Uani 1 6 d S . .
B1 B 0.1829(10) 0.366(2) 0.277(3) 0.013(2) Uani 1 2 d SU . .
O1 O -0.0930(10) 0.6028(10) 0.6880(13) 0.022(2) Uani 1 1 d . . .
O2 O 0.1595(8) 0.3190(16) 0.451(2) 0.031(4) Uani 1 2 d S . .
O3 O 0.4086(10) 0.817(2) -0.199(3) 0.059(2) Uani 1 2 d SU . .
O4 O 0.3333 0.6667 -0.504(4) 0.014(4) Uani 1 6 d S . .
Br1 Br 1.0000 1.0000 0.1072(5) 0.0191(6) Uani 1 6 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Br Br -0.2901 2.4595 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 Ba1 O3 148.3(4) 1_556 2_665
O4 Ba1 O3 148.3(4) 1_556 .
O3 Ba1 O3 54.1(7) 2_665 .
O4 Ba1 O3 148.3(4) 1_556 3_565
O3 Ba1 O3 54.1(7) 2_665 3_565
O3 Ba1 O3 54.1(7) . 3_565
O4 Ba1 O1 81.13(18) 1_556 12_554
O3 Ba1 O1 73.1(4) 2_665 12_554
O3 Ba1 O1 94.60(19) . 12_554
O3 Ba1 O1 127.1(4) 3_565 12_554
O4 Ba1 O1 81.13(18) 1_556 6_664
O3 Ba1 O1 94.60(19) 2_665 6_664
O3 Ba1 O1 73.1(4) . 6_664
O3 Ba1 O1 127.1(4) 3_565 6_664
O1 Ba1 O1 48.1(4) 12_554 6_664
O4 Ba1 O1 81.13(18) 1_556 4_564
O3 Ba1 O1 73.1(4) 2_665 4_564
O3 Ba1 O1 127.1(4) . 4_564
O3 Ba1 O1 94.60(19) 3_565 4_564
O1 Ba1 O1 70.3(4) 12_554 4_564
O1 Ba1 O1 117.67(10) 6_664 4_564
O4 Ba1 O1 81.13(18) 1_556 10_564
O3 Ba1 O1 127.1(4) 2_665 10_564
O3 Ba1 O1 73.1(4) . 10_564
O3 Ba1 O1 94.60(19) 3_565 10_564
O1 Ba1 O1 117.67(9) 12_554 10_564
O1 Ba1 O1 70.3(4) 6_664 10_564
O1 Ba1 O1 159.0(4) 4_564 10_564
O4 Ba1 O1 81.13(18) 1_556 11_664
O3 Ba1 O1 94.60(19) 2_665 11_664
O3 Ba1 O1 127.1(4) . 11_664
O3 Ba1 O1 73.1(4) 3_565 11_664
O1 Ba1 O1 117.67(10) 12_554 11_664
O1 Ba1 O1 159.0(4) 6_664 11_664
O1 Ba1 O1 48.1(3) 4_564 11_664
O1 Ba1 O1 117.67(10) 10_564 11_664
O4 Ba1 O1 81.13(18) 1_556 5_554
O3 Ba1 O1 127.1(4) 2_665 5_554
O3 Ba1 O1 94.60(19) . 5_554
O3 Ba1 O1 73.1(4) 3_565 5_554
O1 Ba1 O1 159.0(4) 12_554 5_554
O1 Ba1 O1 117.67(10) 6_664 5_554
O1 Ba1 O1 117.67(9) 4_564 5_554
O1 Ba1 O1 48.1(3) 10_564 5_554
O1 Ba1 O1 70.3(4) 11_664 5_554
O4 Ba1 B1 69.4(4) 1_556 3_565
O3 Ba1 B1 93.1(4) 2_665 3_565
O3 Ba1 B1 93.1(4) . 3_565
O3 Ba1 B1 142.3(5) 3_565 3_565
O1 Ba1 B1 26.3(2) 12_554 3_565
O1 Ba1 B1 26.3(2) 6_664 3_565
O1 Ba1 B1 92.10(19) 4_564 3_565
O1 Ba1 B1 92.10(19) 10_564 3_565
O1 Ba1 B1 134.2(3) 11_664 3_565
O1 Ba1 B1 134.2(3) 5_554 3_565
O4 Ba1 B1 69.4(4) 1_556 2_665
O3 Ba1 B1 142.3(5) 2_665 2_665
O3 Ba1 B1 93.1(4) . 2_665
O3 Ba1 B1 93.1(4) 3_565 2_665
O1 Ba1 B1 134.2(3) 12_554 2_665
O1 Ba1 B1 92.10(19) 6_664 2_665
O1 Ba1 B1 134.2(3) 4_564 2_665
O1 Ba1 B1 26.3(2) 10_564 2_665
O1 Ba1 B1 92.10(19) 11_664 2_665
O1 Ba1 B1 26.3(2) 5_554 2_665
B1 Ba1 B1 108.3(4) 3_565 2_665
O2 Ba2 O1 69.09(17) 2_664 8_554
O2 Ba2 O1 69.09(17) 2_664 3_564
O1 Ba2 O1 138.2(3) 8_554 3_564
O2 Ba2 O1 144.6(3) 2_664 5_554
O1 Ba2 O1 85.5(2) 8_554 5_554
O1 Ba2 O1 130.5(3) 3_564 5_554
O2 Ba2 O1 144.6(3) 2_664 10_564
O1 Ba2 O1 130.5(3) 8_554 10_564
O1 Ba2 O1 85.5(2) 3_564 10_564
O1 Ba2 O1 45.8(3) 5_554 10_564
O2 Ba2 O2 108.8(3) 2_664 4_664
O1 Ba2 O2 46.3(3) 8_554 4_664
O1 Ba2 O2 158.4(3) 3_564 4_664
O1 Ba2 O2 64.0(3) 5_554 4_664
O1 Ba2 O2 103.7(3) 10_564 4_664
O2 Ba2 O2 108.8(3) 2_664 6_664
O1 Ba2 O2 158.4(3) 8_554 6_664
O1 Ba2 O2 46.3(3) 3_564 6_664
O1 Ba2 O2 103.7(3) 5_554 6_664
O1 Ba2 O2 64.0(3) 10_564 6_664
O2 Ba2 O2 120.4(5) 4_664 6_664
O2 Ba2 O3 80.7(5) 2_664 3_565
O1 Ba2 O3 64.1(4) 8_554 3_565
O1 Ba2 O3 107.6(4) 3_564 3_565
O1 Ba2 O3 65.8(4) 5_554 3_565
O1 Ba2 O3 84.2(4) 10_564 3_565
O2 Ba2 O3 92.9(4) 4_664 3_565
O2 Ba2 O3 137.5(4) 6_664 3_565
O2 Ba2 O3 80.7(5) 2_664 .
O1 Ba2 O3 107.6(4) 8_554 .
O1 Ba2 O3 64.1(4) 3_564 .
O1 Ba2 O3 84.2(4) 5_554 .
O1 Ba2 O3 65.8(4) 10_564 .
O2 Ba2 O3 137.5(4) 4_664 .
O2 Ba2 O3 92.9(4) 6_664 .
O3 Ba2 O3 46.6(7) 3_565 .
O2 Ba2 Br1 65.8(3) 2_664 4_774
O1 Ba2 Br1 82.17(18) 8_554 4_774
O1 Ba2 Br1 82.17(18) 3_564 4_774
O1 Ba2 Br1 136.5(2) 5_554 4_774
O1 Ba2 Br1 136.5(2) 10_564 4_774
O2 Ba2 Br1 77.7(3) 4_664 4_774
O2 Ba2 Br1 77.7(3) 6_664 4_774
O3 Ba2 Br1 139.3(4) 3_565 4_774
O3 Ba2 Br1 139.3(4) . 4_774
O2 Ba2 B1 85.0(4) 2_664 4_664
O1 Ba2 B1 25.1(3) 8_554 4_664
O1 Ba2 B1 148.4(4) 3_564 4_664
O1 Ba2 B1 81.1(4) 5_554 4_664
O1 Ba2 B1 125.3(4) 10_564 4_664
O2 Ba2 B1 24.1(4) 4_664 4_664
O2 Ba2 B1 136.0(4) 6_664 4_664
O3 Ba2 B1 84.9(4) 3_565 4_664
O3 Ba2 B1 130.9(4) . 4_664
Br1 Ba2 B1 70.4(3) 4_774 4_664
O2 Ba2 B1 85.0(4) 2_664 6_664
O1 Ba2 B1 148.4(4) 8_554 6_664
O1 Ba2 B1 25.1(3) 3_564 6_664
O1 Ba2 B1 125.3(4) 5_554 6_664
O1 Ba2 B1 81.1(4) 10_564 6_664
O2 Ba2 B1 136.0(4) 4_664 6_664
O2 Ba2 B1 24.1(4) 6_664 6_664
O3 Ba2 B1 130.9(4) 3_565 6_664
O3 Ba2 B1 84.9(4) . 6_664
Br1 Ba2 B1 70.4(3) 4_774 6_664
B1 Ba2 B1 140.3(6) 4_664 6_664
O3 Ba3 O1 76.7(4) 2_666 .
O3 Ba3 O1 76.7(4) 2_666 9_565
O1 Ba3 O1 79.0(4) . 9_565
O3 Ba3 O3 149.8(6) 2_666 5_455
O1 Ba3 O3 80.0(4) . 5_455
O1 Ba3 O3 80.0(4) 9_565 5_455
O3 Ba3 O4 59.4(7) 2_666 1_556
O1 Ba3 O4 121.2(4) . 1_556
O1 Ba3 O4 121.2(4) 9_565 1_556
O3 Ba3 O4 150.9(7) 5_455 1_556
O3 Ba3 O1 127.8(3) 2_666 12_554
O1 Ba3 O1 97.5(3) . 12_554
O1 Ba3 O1 154.1(2) 9_565 12_554
O3 Ba3 O1 74.1(4) 5_455 12_554
O4 Ba3 O1 82.8(5) 1_556 12_554
O3 Ba3 O1 127.8(3) 2_666 4_564
O1 Ba3 O1 154.1(2) . 4_564
O1 Ba3 O1 97.5(3) 9_565 4_564
O3 Ba3 O1 74.1(4) 5_455 4_564
O4 Ba3 O1 82.8(5) 1_556 4_564
O1 Ba3 O1 74.4(4) 12_554 4_564
O3 Ba3 O2 84.7(3) 2_666 3_565
O1 Ba3 O2 68.2(3) . 3_565
O1 Ba3 O2 145.3(3) 9_565 3_565
O3 Ba3 O2 104.3(3) 5_455 3_565
O4 Ba3 O2 70.5(2) 1_556 3_565
O1 Ba3 O2 47.1(3) 12_554 3_565
O1 Ba3 O2 116.9(3) 4_564 3_565
O3 Ba3 O2 84.7(3) 2_666 .
O1 Ba3 O2 145.3(3) . .
O1 Ba3 O2 68.2(3) 9_565 .
O3 Ba3 O2 104.3(3) 5_455 .
O4 Ba3 O2 70.5(2) 1_556 .
O1 Ba3 O2 116.9(3) 12_554 .
O1 Ba3 O2 47.1(3) 4_564 .
O2 Ba3 O2 139.4(4) 3_565 .
O3 Ba3 B1 102.7(4) 2_666 3_565
O1 Ba3 B1 88.6(4) . 3_565
O1 Ba3 B1 167.3(4) 9_565 3_565
O3 Ba3 B1 95.8(4) 5_455 3_565
O4 Ba3 B1 67.4(4) 1_556 3_565
O1 Ba3 B1 25.4(3) 12_554 3_565
O1 Ba3 B1 92.7(4) 4_564 3_565
O2 Ba3 B1 24.4(4) 3_565 3_565
O2 Ba3 B1 124.4(4) . 3_565
O3 Ba3 Si1 29.2(5) 2_666 1_556
O1 Ba3 Si1 99.2(3) . 1_556
O1 Ba3 Si1 99.2(3) 9_565 1_556
O3 Ba3 Si1 179.0(4) 5_455 1_556
O4 Ba3 Si1 30.1(5) 1_556 1_556
O1 Ba3 Si1 106.7(2) 12_554 1_556
O1 Ba3 Si1 106.7(2) 4_564 1_556
O2 Ba3 Si1 75.9(3) 3_565 1_556
O2 Ba3 Si1 75.9(3) . 1_556
B1 Ba3 Si1 84.8(3) 3_565 1_556
O3 Ba3 Ba3 166.2(4) 2_666 4_564
O1 Ba3 Ba3 113.5(2) . 4_564
O1 Ba3 Ba3 113.5(2) 9_565 4_564
O3 Ba3 Ba3 44.0(4) 5_455 4_564
O4 Ba3 Ba3 106.8(5) 1_556 4_564
O1 Ba3 Ba3 44.20(18) 12_554 4_564
O1 Ba3 Ba3 44.20(18) 4_564 4_564
O2 Ba3 Ba3 90.5(3) 3_565 4_564
O2 Ba3 Ba3 90.5(3) . 4_564
B1 Ba3 Ba3 69.5(3) 3_565 4_564
Si1 Ba3 Ba3 136.96(16) 1_556 4_564
O3 Si1 O3 106.3(9) . 2_665
O3 Si1 O3 106.3(9) . 3_565
O3 Si1 O3 106.3(9) 2_665 3_565
O3 Si1 O4 112.5(8) . .
O3 Si1 O4 112.5(8) 2_665 .
O3 Si1 O4 112.5(8) 3_565 .
O3 Si1 Ba3 126.4(3) . 1_554
O3 Si1 Ba3 54.1(7) 2_665 1_554
O3 Si1 Ba3 126.4(3) 3_565 1_554
O4 Si1 Ba3 58.36(16) . 1_554
O3 Si1 Ba3 54.1(7) . 3_564
O3 Si1 Ba3 126.4(3) 2_665 3_564
O3 Si1 Ba3 126.4(3) 3_565 3_564
O4 Si1 Ba3 58.36(16) . 3_564
Ba3 Si1 Ba3 95.0(2) 1_554 3_564
O3 Si1 Ba3 126.4(3) . 2_664
O3 Si1 Ba3 126.4(3) 2_665 2_664
O3 Si1 Ba3 54.1(7) 3_565 2_664
O4 Si1 Ba3 58.36(16) . 2_664
Ba3 Si1 Ba3 95.0(2) 1_554 2_664
Ba3 Si1 Ba3 95.0(2) 3_564 2_664
O3 Si1 Ba2 57.67(6) . 2_665
O3 Si1 Ba2 57.67(6) 2_665 2_665
O3 Si1 Ba2 144.8(9) 3_565 2_665
O4 Si1 Ba2 102.70(15) . 2_665
Ba3 Si1 Ba2 72.55(3) 1_554 2_665
Ba3 Si1 Ba2 72.55(3) 3_564 2_665
Ba3 Si1 Ba2 161.1(3) 2_664 2_665
O3 Si1 Ba2 144.8(9) . 3_565
O3 Si1 Ba2 57.67(6) 2_665 3_565
O3 Si1 Ba2 57.67(6) 3_565 3_565
O4 Si1 Ba2 102.70(15) . 3_565
Ba3 Si1 Ba2 72.55(3) 1_554 3_565
Ba3 Si1 Ba2 161.1(3) 3_564 3_565
Ba3 Si1 Ba2 72.55(3) 2_664 3_565
Ba2 Si1 Ba2 115.31(11) 2_665 3_565
O2 B1 O1 121.1(8) . 4_564
O2 B1 O1 121.1(8) . 11_664
O1 B1 O1 117.5(17) 4_564 11_664
O2 B1 Ba1 130.4(13) . .
O1 B1 Ba1 68.2(9) 4_564 .
O1 B1 Ba1 68.2(9) 11_664 .
O2 B1 Ba3 73.7(7) . 2_665
O1 B1 Ba3 138.2(12) 4_564 2_665
O1 B1 Ba3 59.0(7) 11_664 2_665
Ba1 B1 Ba3 73.4(4) . 2_665
O2 B1 Ba2 70.5(7) . 4_665
O1 B1 Ba2 146.9(12) 4_564 4_665
O1 B1 Ba2 64.1(6) 11_664 4_665
Ba1 B1 Ba2 131.0(3) . 4_665
Ba3 B1 Ba2 73.18(16) 2_665 4_665
O2 B1 Ba2 70.5(7) . 5_455
O1 B1 Ba2 64.1(6) 4_564 5_455
O1 B1 Ba2 146.9(12) 11_664 5_455
Ba1 B1 Ba2 131.0(3) . 5_455
Ba3 B1 Ba2 144.1(7) 2_665 5_455
Ba2 B1 Ba2 96.4(5) 4_665 5_455
O2 B1 Ba2 147.4(13) . 3_565
O1 B1 Ba2 65.8(9) 4_564 3_565
O1 B1 Ba2 65.8(9) 11_664 3_565
Ba1 B1 Ba2 82.2(5) . 3_565
Ba3 B1 Ba2 124.6(4) 2_665 3_565
Ba2 B1 Ba2 88.4(4) 4_665 3_565
Ba2 B1 Ba2 88.4(4) 5_455 3_565
B1 O1 Ba3 172.4(10) 4_565 .
B1 O1 Ba3 95.6(9) 4_565 4_565
Ba3 O1 Ba3 88.6(3) . 4_565
B1 O1 Ba1 85.6(9) 4_565 4_565
Ba3 O1 Ba1 88.6(3) . 4_565
Ba3 O1 Ba1 83.7(3) 4_565 4_565
B1 O1 Ba2 90.8(9) 4_565 2_666
Ba3 O1 Ba2 95.9(3) . 2_666
Ba3 O1 Ba2 85.1(3) 4_565 2_666
Ba1 O1 Ba2 167.9(4) 4_565 2_666
B1 O1 Ba2 89.6(9) 4_565 6
Ba3 O1 Ba2 85.6(3) . 6
Ba3 O1 Ba2 172.3(4) 4_565 6
Ba1 O1 Ba2 91.0(3) 4_565 6
Ba2 O1 Ba2 100.5(3) 2_666 6
B1 O2 Ba2 166.0(13) . 3_566
B1 O2 Ba2 85.4(7) . 4_665
Ba2 O2 Ba2 103.0(3) 3_566 4_665
B1 O2 Ba2 85.4(7) . 5_455
Ba2 O2 Ba2 103.0(3) 3_566 5_455
Ba2 O2 Ba2 104.1(5) 4_665 5_455
B1 O2 Ba3 81.9(7) . 2_665
Ba2 O2 Ba3 89.1(4) 3_566 2_665
Ba2 O2 Ba3 77.02(5) 4_665 2_665
Ba2 O2 Ba3 167.2(5) 5_455 2_665
B1 O2 Ba3 81.9(7) . .
Ba2 O2 Ba3 89.1(4) 3_566 .
Ba2 O2 Ba3 167.2(5) 4_665 .
Ba2 O2 Ba3 77.02(5) 5_455 .
Ba3 O2 Ba3 99.1(5) 2_665 .
Si1 O3 Ba3 96.6(9) . 3_564
Si1 O3 Ba3 171.9(12) . 6_664
Ba3 O3 Ba3 91.5(6) 3_564 6_664
Si1 O3 Ba1 80.8(8) . .
Ba3 O3 Ba1 177.4(8) 3_564 .
Ba3 O3 Ba1 91.0(6) 6_664 .
Si1 O3 Ba2 97.6(3) . 2_665
Ba3 O3 Ba2 90.2(4) 3_564 2_665
Ba3 O3 Ba2 82.3(3) 6_664 2_665
Ba1 O3 Ba2 90.1(4) . 2_665
Si1 O3 Ba2 97.6(4) . .
Ba3 O3 Ba2 90.2(4) 3_564 .
Ba3 O3 Ba2 82.3(3) 6_664 .
Ba1 O3 Ba2 90.1(4) . .
Ba2 O3 Ba2 164.6(7) 2_665 .
Si1 O4 Ba1 180.000(1) . 1_554
Si1 O4 Ba3 91.5(5) . 1_554
Ba1 O4 Ba3 88.5(5) 1_554 1_554
Si1 O4 Ba3 91.5(5) . 3_564
Ba1 O4 Ba3 88.5(5) 1_554 3_564
Ba3 O4 Ba3 119.93(5) 1_554 3_564
Si1 O4 Ba3 91.5(5) . 2_664
Ba1 O4 Ba3 88.5(5) 1_554 2_664
Ba3 O4 Ba3 119.93(5) 1_554 2_664
Ba3 O4 Ba3 119.93(5) 3_564 2_664
Ba2 Br1 Ba2 97.08(8) 4_775 6_655
Ba2 Br1 Ba2 97.08(8) 4_775 5_565
Ba2 Br1 Ba2 97.08(8) 6_655 5_565
Ba2 Br1 Ba2 174.53(11) 4_775 .
Ba2 Br1 Ba2 86.51(3) 6_655 .
Ba2 Br1 Ba2 86.51(3) 5_565 .
Ba2 Br1 Ba2 86.51(3) 4_775 3_675
Ba2 Br1 Ba2 174.53(11) 6_655 3_675
Ba2 Br1 Ba2 86.51(3) 5_565 3_675
Ba2 Br1 Ba2 89.61(8) . 3_675
Ba2 Br1 Ba2 86.51(3) 4_775 2_765
Ba2 Br1 Ba2 86.51(3) 6_655 2_765
Ba2 Br1 Ba2 174.53(11) 5_565 2_765
Ba2 Br1 Ba2 89.61(8) . 2_765
Ba2 Br1 Ba2 89.61(8) 3_675 2_765
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 O4 2.71(3) 1_556
Ba1 O3 2.80(2) 2_665
Ba1 O3 2.80(2) .
Ba1 O3 2.80(2) 3_565
Ba1 O1 2.924(10) 12_554
Ba1 O1 2.924(10) 6_664
Ba1 O1 2.924(11) 4_564
Ba1 O1 2.924(11) 10_564
Ba1 O1 2.924(10) 11_664
Ba1 O1 2.924(10) 5_554
Ba1 B1 3.14(2) 3_565
Ba1 B1 3.14(2) 2_665
Ba2 O2 2.800(15) 2_664
Ba2 O1 2.959(11) 8_554
Ba2 O1 2.959(11) 3_564
Ba2 O1 3.059(9) 5_554
Ba2 O1 3.059(9) 10_564
Ba2 O2 3.110(11) 4_664
Ba2 O2 3.110(11) 6_664
Ba2 O3 3.217(17) 3_565
Ba2 O3 3.217(16) .
Ba2 Br1 3.272(2) 4_774
Ba2 B1 3.289(13) 4_664
Ba2 B1 3.289(13) 6_664
Ba3 O3 2.64(2) 2_666
Ba3 O1 2.648(9) .
Ba3 O1 2.648(9) 9_565
Ba3 O3 2.66(2) 5_455
Ba3 O4 2.7556(14) 1_556
Ba3 O1 2.786(9) 12_554
Ba3 O1 2.786(9) 4_564
Ba3 O2 3.136(11) 3_565
Ba3 O2 3.136(11) .
Ba3 B1 3.235(14) 3_565
Ba3 Si1 3.236(6) 1_556
Ba3 Ba3 3.7967(19) 4_564
Si1 O3 1.59(2) .
Si1 O3 1.59(2) 2_665
Si1 O3 1.59(2) 3_565
Si1 O4 1.62(3) .
Si1 Ba3 3.236(6) 1_554
Si1 Ba3 3.236(6) 3_564
Si1 Ba3 3.236(6) 2_664
Si1 Ba2 3.773(3) 2_665
Si1 Ba2 3.773(3) 3_565
B1 O2 1.35(2) .
B1 O1 1.394(13) 4_564
B1 O1 1.394(13) 11_664
B1 Ba3 3.235(14) 2_665
B1 Ba2 3.289(13) 4_665
B1 Ba2 3.289(13) 5_455
B1 Ba2 3.35(2) 3_565
O1 B1 1.394(13) 4_565
O1 Ba3 2.786(9) 4_565
O1 Ba1 2.924(10) 4_565
O1 Ba2 2.959(11) 2_666
O1 Ba2 3.059(9) 6
O2 Ba2 2.800(15) 3_566
O2 Ba2 3.110(11) 4_665
O2 Ba2 3.110(11) 5_455
O2 Ba3 3.136(11) 2_665
O3 Ba3 2.64(2) 3_564
O3 Ba3 2.66(2) 6_664
O3 Ba2 3.217(16) 2_665
O4 Ba1 2.71(3) 1_554
O4 Ba3 2.7556(14) 1_554
O4 Ba3 2.7556(14) 3_564
O4 Ba3 2.7556(14) 2_664
Br1 Ba2 3.272(2) 4_775
Br1 Ba2 3.272(2) 6_655
Br1 Ba2 3.272(2) 5_565
Br1 Ba2 3.479(3) 3_675
Br1 Ba2 3.479(3) 2_765
